- Project plans
- Project activities
- Legislation and standards
- Industry context
Last edited 22 Jun 2018
Efflorescence is a crystalline, salty deposit that can occur on the surfaces of bricks, masonry or concrete. It is generally a white or off-white colour with a powdery appearance. While not a risk structurally, it affects the appearance of a building, particularly it features coloured concrete or brickwork.
- Low temperatures.
- Moist conditions.
- Rain or dew.
- Water added to the surface of fresh concrete to aid the troweling process.
Water moves and migrates through capillaries (channels) in concrete, masonry, mortar or brickwork, carrying salts to the surface. The fewer capillaries there are, or the higher the density of the material, the more difficulty the water will have in passing through to the surface. The higher the porosity of the material, the greater the likelihood of efflorescence occurring.
Calcium hydroxide, which is formed in the hydration reaction of Portland cement, is carried through the capillaries to the surface by water. On reaching the surface, it combines with carbon dioxide from the air to produce calcium carbonate and water, which evaporates leaving the salt deposits. Hydroxides and sulfates of either sodium or potassium can also cause efflorescence, and as these are more water soluble than calcium, tend to appear much more quickly. These salts tend to come from cement, aggregates or admixtures.
Low humidity can result in the evaporation of water prior to reaching the structure's surface, which means that the salt deposit remains unseen. High humidity can result in slower evaporation and hence more opportunity for growth of the deposits. Efflorescence is often more of a problem after periods of consistent or heavy rain, but less so in dryer summer periods.
 Preventing efflorescence
Steps can be taken to prevent or limit the spread of efflorescence. For example, in their natural state sand and gravel may have been associated with salt-bearing water or soil. This can lead to efflorescence unless the salts are removed by washing. This procedure is common practice for many suppliers so the risk should be small.
Mixing-water used for mortar or concrete may be taken from a natural source which has been in contact with a sulfate-bearing soil. In this instance, efflorescence can be reduced by using a low water-cement ratio mix for concreting.
Clay products such as building bricks and face bricks may also contain soluble salts. To prevent or reduce this, the clay can be washed during the manufacturing process, and a barium salt (such as barium carbonate) added to react with the calcium sulfate. This reaction results in the compounds barium sulfate and calcium carbonate, both of which are fairly insoluble.
In terms of site storage, bricks should be kept off the ground in a dry place so as to prevent dampness or the absorption of moisture. A test can be carried out to ascertain the soluble salt content of a batch of bricks. One brick is placed in distilled water for a week, after which the extent to which the water has been drawn through the brick and evaporated from the surface should be evident.
 Removing efflorescence
There are a number of methods for removing efflorescence effectively.
Calcium hydroxide can be removed before it combines with carbon dioxide by either pressure washing or wet-scrubbing which puts it in solution with water and allows it to be rinsed away. Fresh water should then be applied by using an air jet or wet vacuum so that the structure isn't left with residue on the surface.
Efflorescence, once it becomes insoluble, is more difficult to remove. A mild acid solution can be applied, often using muriatic acid which has been diluted from full strength. After acid washing, the surface should be thoroughly flushed with water and neutralised with baking soda or an equivalent form of sodium bicarbonate. It is important to consider the implications of using acid on the structure surface, which can erode mortar and discolour brickwork.
Light sandblasting can be used for efflorescence that has been present for several months. Once the surface is dry, the application of a stiff brush to the surface can help to prevent the salt from penetrating again.
 Related articles on Designing Buildings Wiki
- Alkali-aggregate reaction (AAR).
- Alkali-silica reaction (ASR).
- Cracking and building movement.
- Defects in brickwork.
- Defects in stonework.
- Diagnosing the causes of dampness (GR 5 revised).
- How to clean masonry.
- Lime run-off.
- Mould growth in buildings.
- Penetrating damp.
- Rising damp.
- Rising damp in walls - diagnosis and treatment (DG 245).
- Wall tie failure.
 External references
- Delaware Quarries - Efflorescence
- Concrete Constructon - What causes efflorescence and how do you remove it?
Featured articles and news
Which room is the most fun to design? Find out the 'Grand Designs' presenter's unusual choice in our interview.
Full suite of speakers are announced for this year's BSRIA Briefing event.
Book your place for the Architectural Technology Awards 2018.
There are many ways of classifying types of building. Have a look at our range of building articles.
BSRIA have launched the 'major update' of the go-to design framework guide for building services.
How to get results with building life cycle assessment.
Government publishes a prospectus inviting proposals for new 'garden communities'.
The Morandi motorway bridge in Genoa collapses during rainstorm while undergoing maintenance works.
'Developed design' is a phrase coined by the RIBA for their 2013 Plan of Work. But what does it actually mean?
New green paper published aiming to rebalance the relationship between landlords and residents and tackle stigma.
RIBA calls for a comprehensive ban on combustible materials.